# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_cvo_mn
_database_code_depnum_ccdc_archive 'CCDC 2111538'
loop_
_audit_author_name
_audit_author_address
'Vladimir Lazarenko'
;NRC Kurchatov institute
Russia
;
_audit_update_record             
;
2021-09-23 deposited with the CCDC.	2022-03-23 downloaded from the CCDC.
;
_audit_creation_date             2021-09-20
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.05(Ca63.3 O168 V42)'
_chemical_formula_sum            'Ca3.01 O8 V2'
_chemical_formula_weight         350.64
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2664 0.3894 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0148 0.0078 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3517 0.6680 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      trigonal
_space_group_IT_number           161
_space_group_name_H-M_alt        'R 3 c'
_space_group_name_Hall           'R 3 -2"c'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+y, y, z+1/2'
'x, x-y, z+1/2'
'-y, -x, z+1/2'
'-x+y, -x, z'
'-y, x-y, z'
'x+2/3, y+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+5/6'
'x+2/3, x-y+1/3, z+5/6'
'-y+2/3, -x+1/3, z+5/6'
'-x+y+2/3, -x+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+7/6'
'x+1/3, x-y+2/3, z+7/6'
'-y+1/3, -x+2/3, z+7/6'
'-x+y+1/3, -x+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'

_cell_length_a                   10.6320(2)
_cell_length_b                   10.6320(2)
_cell_length_c                   37.3860(13)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     3659.90(19)
_cell_formula_units_Z            21
_cell_measurement_reflns_used    500
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      31.871
_cell_measurement_theta_min      2.613
_shelx_estimated_absorpt_T_max   0.348
_shelx_estimated_absorpt_T_min   0.348
_exptl_absorpt_coefficient_mu    6.693
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.437
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'XDS (Kabsh, 2010)'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.341
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             3575
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0473
_diffrn_reflns_av_unetI/netI     0.0524
_diffrn_reflns_Laue_measured_fraction_full 0.981
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       50
_diffrn_reflns_limit_l_min       -52
_diffrn_reflns_number            6708
_diffrn_reflns_point_group_measured_fraction_full 0.962
_diffrn_reflns_point_group_measured_fraction_max 0.955
_diffrn_reflns_theta_full        26.867
_diffrn_reflns_theta_max         31.871
_diffrn_reflns_theta_min         2.613
_diffrn_ambient_temperature      100.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Rayonix SX165 CCD'
_diffrn_measurement_method       '/f scan'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.7532
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.931
_reflns_Friedel_fraction_full    0.942
_reflns_Friedel_fraction_max     0.924
_reflns_number_gt                2229
_reflns_number_total             2261
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         1.231
_refine_diff_density_min         -0.992
_refine_diff_density_rms         0.164
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.39(5)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     149
_refine_ls_number_reflns         2249
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0409
_refine_ls_R_factor_gt           0.0403
_refine_ls_restrained_S_all      1.050
_refine_ls_shift/su_max          0.047
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0563P)²+36.9246P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1050
_refine_ls_wR_factor_ref         0.1073
_refine_special_details          'Refined as a 2-component inversion twin.,Twin'
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.61(6)
 0.39(6)
2. Uiso/Uaniso restraints and constraints
Uanis(Ca5A) = Uanis(Ca5)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ca1 Ca 0.14743(17) 0.27017(19) 0.55698(5) 0.0251(4) Uani 1 1 d . . . . .
Ca2 Ca -0.19634(15) 0.19630(15) 0.49701(4) 0.0170(3) Uani 1 1 d . . . . .
Ca3 Ca 0.51066(15) 0.45674(15) 0.63252(4) 0.0159(3) Uani 1 1 d . . . . .
Ca4 Ca 0.666667 0.333333 0.56781(7) 0.0187(4) Uani 1 3 d S T P . .
Ca5 Ca -0.0156(12) -0.0680(17) 0.4221(3) 0.036(3) Uani 0.168(9) 1 d . . . A 1
V1 V 0.47056(15) 0.49302(14) 0.53420(3) 0.0202(3) Uani 1 1 d . . . . .
V2 V 0.81663(12) 0.68289(13) 0.59855(3) 0.0144(2) Uani 1 1 d . . . . .
V3 V 0.000000 0.000000 0.49990(5) 0.0141(4) Uani 1 3 d S T P A .
O1 O 0.4118(12) 0.4691(10) 0.57626(19) 0.057(3) Uani 1 1 d . . . . .
O2 O 0.5636(8) 0.6669(6) 0.52085(18) 0.0333(14) Uani 1 1 d . . . . .
O3 O 0.3217(5) 0.3752(5) 0.51057(13) 0.0149(8) Uani 1 1 d . . . . .
O4 O 0.5849(7) 0.4265(8) 0.5262(3) 0.044(2) Uani 1 1 d . . . . .
O5 O 0.8469(7) 0.7071(8) 0.55476(16) 0.0275(13) Uani 1 1 d . . . . .
O6 O 0.6993(8) 0.7380(7) 0.60885(15) 0.0339(14) Uani 1 1 d . . . . .
O7 O 0.9815(9) 0.7660(9) 0.6170(2) 0.0454(18) Uani 1 1 d . . . . .
O8 O 0.7428(5) 0.5072(6) 0.61044(14) 0.0183(9) Uani 1 1 d . . . . .
O9 O 0.000000 0.000000 0.5443(3) 0.037(3) Uani 1 3 d S T P A .
O10 O 0.1462(6) -0.0095(7) 0.48691(19) 0.0308(13) Uani 1 1 d . . . . .
Ca5A Ca 0.000000 0.000000 0.407(6) 0.036(7) Uani 0.018(12) 3 d S T P A 2


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ca1 V1 3.163(2) . ?
Ca1 V2 3.223(2) 6_655 ?
Ca1 V2 3.0732(18) 5_565 ?
Ca1 O1 2.636(11) . ?
Ca1 O2 2.449(6) 5_565 ?
Ca1 O3 2.371(5) . ?
Ca1 O5 2.542(7) 6_655 ?
Ca1 O5 2.661(6) 5_565 ?
Ca1 O6 2.362(6) 5_565 ?
Ca1 O7 2.598(9) 6_655 ?
Ca1 O9 2.536(3) . ?
Ca1 O10 2.951(8) 6 ?
Ca2 V1 3.1553(19) 6 ?
Ca2 V1 3.413(2) 5_565 ?
Ca2 V2 3.5168(19) 8_444 ?
Ca2 V3 3.6168(13) . ?
Ca2 O2 3.055(8) 5_565 ?
Ca2 O3 2.424(5) 6 ?
Ca2 O4 2.415(8) 5_565 ?
Ca2 O4 2.522(8) 6 ?
Ca2 O5 2.347(7) 5_565 ?
Ca2 O6 2.381(6) 8_444 ?
Ca2 O7 2.267(8) 10_564 ?
Ca2 O10 2.462(6) 6 ?
Ca3 Ca4 3.536(2) . ?
Ca3 Ca5 3.543(12) 16_554 ?
Ca3 V2 3.2518(19) 6_655 ?
Ca3 V2 3.1867(18) . ?
Ca3 O1 2.384(8) . ?
Ca3 O2 2.351(7) 14_544 ?
Ca3 O3 2.316(5) 15_554 ?
Ca3 O6 2.784(7) . ?
Ca3 O7 2.832(9) 6_655 ?
Ca3 O8 2.408(5) 6_655 ?
Ca3 O8 2.395(5) . ?
Ca3 O10 2.339(6) 16_554 ?
Ca4 V1 3.5141(16) 6_655 ?
Ca4 V1 3.5141(16) 5_665 ?
Ca4 V1 3.5140(16) . ?
Ca4 V2 3.4278(14) 5_665 ?
Ca4 V2 3.4278(14) . ?
Ca4 V2 3.4278(15) 6_655 ?
Ca4 O4 2.240(7) 6_655 ?
Ca4 O4 2.240(7) . ?
Ca4 O4 2.240(7) 5_665 ?
Ca4 O8 2.262(6) . ?
Ca4 O8 2.262(6) 6_655 ?
Ca4 O8 2.262(6) 5_665 ?
Ca5 Ca5 1.14(3) 5 ?
Ca5 Ca5 1.14(3) 6 ?
Ca5 V1 3.199(10) 10_554 ?
Ca5 V1 3.429(11) 8_444 ?
Ca5 V3 2.980(11) . ?
Ca5 O1 2.371(14) 10_554 ?
Ca5 O1 2.444(16) 8_444 ?
Ca5 O2 3.120(14) 10_554 ?
Ca5 O6 3.011(17) 10_554 ?
Ca5 O10 2.853(13) . ?
Ca5 O10 2.745(13) 5 ?
V1 O1 1.664(8) . ?
V1 O2 1.679(6) . ?
V1 O3 1.695(5) . ?
V1 O4 1.710(8) . ?
V1 Ca5A 3.22(11) 14_554 ?
V2 O5 1.664(6) . ?
V2 O6 1.667(6) . ?
V2 O7 1.668(8) . ?
V2 O8 1.684(5) . ?
V3 O9 1.658(11) . ?
V3 O10 1.679(5) 6 ?
V3 O10 1.679(5) . ?
V3 O10 1.679(5) 5 ?
O1 Ca5A 2.622(14) 14_554 ?
O2 Ca5A 3.14(15) 14_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
V1 Ca1 V2 79.88(5) . 6_655 ?
V2 Ca1 V1 152.92(8) 5_565 . ?
V2 Ca1 V2 107.48(6) 5_565 6_655 ?
O1 Ca1 V1 31.72(17) . . ?
O1 Ca1 V2 126.1(2) . 5_565 ?
O1 Ca1 V2 67.5(2) . 6_655 ?
O1 Ca1 O5 153.9(3) . 5_565 ?
O1 Ca1 O10 133.2(2) . 6 ?
O2 Ca1 V1 80.72(18) 5_565 . ?
O2 Ca1 V2 160.53(19) 5_565 6_655 ?
O2 Ca1 V2 89.28(16) 5_565 5_565 ?
O2 Ca1 O1 94.8(3) 5_565 . ?
O2 Ca1 O5 74.4(2) 5_565 5_565 ?
O2 Ca1 O5 139.8(2) 5_565 6_655 ?
O2 Ca1 O7 148.7(3) 5_565 6_655 ?
O2 Ca1 O9 118.8(3) 5_565 . ?
O2 Ca1 O10 64.7(2) 5_565 6 ?
O3 Ca1 V1 31.77(12) . . ?
O3 Ca1 V2 157.70(13) . 5_565 ?
O3 Ca1 V2 94.79(12) . 6_655 ?
O3 Ca1 O1 63.5(2) . . ?
O3 Ca1 O2 69.07(19) . 5_565 ?
O3 Ca1 O5 71.80(19) . 6_655 ?
O3 Ca1 O5 129.87(19) . 5_565 ?
O3 Ca1 O7 117.2(2) . 6_655 ?
O3 Ca1 O9 106.9(2) . . ?
O3 Ca1 O10 69.80(18) . 6 ?
O5 Ca1 V1 154.78(17) 5_565 . ?
O5 Ca1 V1 70.76(16) 6_655 . ?
O5 Ca1 V2 32.74(13) 5_565 5_565 ?
O5 Ca1 V2 125.04(18) 5_565 6_655 ?
O5 Ca1 V2 128.20(17) 6_655 5_565 ?
O5 Ca1 V2 30.75(14) 6_655 6_655 ?
O5 Ca1 O1 75.6(3) 6_655 . ?
O5 Ca1 O5 127.8(3) 6_655 5_565 ?
O5 Ca1 O7 61.7(2) 6_655 6_655 ?
O5 Ca1 O10 93.35(17) 6_655 6 ?
O5 Ca1 O10 64.02(18) 5_565 6 ?
O6 Ca1 V1 122.77(19) 5_565 . ?
O6 Ca1 V2 32.49(16) 5_565 5_565 ?
O6 Ca1 V2 95.09(17) 5_565 6_655 ?
O6 Ca1 O1 93.7(3) 5_565 . ?
O6 Ca1 O2 94.0(2) 5_565 5_565 ?
O6 Ca1 O3 149.0(2) 5_565 . ?
O6 Ca1 O5 125.1(2) 5_565 6_655 ?
O6 Ca1 O5 64.14(19) 5_565 5_565 ?
O6 Ca1 O7 64.8(2) 5_565 6_655 ?
O6 Ca1 O9 104.0(3) 5_565 . ?
O6 Ca1 O10 127.5(2) 5_565 6 ?
O7 Ca1 V1 91.51(19) 6_655 . ?
O7 Ca1 V2 30.98(16) 6_655 6_655 ?
O7 Ca1 V2 84.06(17) 6_655 5_565 ?
O7 Ca1 O1 65.7(3) 6_655 . ?
O7 Ca1 O5 112.0(2) 6_655 5_565 ?
O7 Ca1 O10 146.4(2) 6_655 6 ?
O9 Ca1 V1 128.51(14) . . ?
O9 Ca1 V2 75.45(15) . 6_655 ?
O9 Ca1 V2 78.30(15) . 5_565 ?
O9 Ca1 O1 140.1(2) . . ?
O9 Ca1 O5 64.94(15) . 6_655 ?
O9 Ca1 O5 63.23(16) . 5_565 ?
O9 Ca1 O7 89.8(3) . 6_655 ?
O9 Ca1 O10 57.9(3) . 6 ?
O10 Ca1 V1 101.51(13) 6 . ?
O10 Ca1 V2 121.12(12) 6 6_655 ?
O10 Ca1 V2 96.71(13) 6 5_565 ?
V1 Ca2 V1 119.80(6) 6 5_565 ?
V1 Ca2 V2 70.08(4) 6 8_444 ?
V1 Ca2 V2 142.61(5) 5_565 8_444 ?
V1 Ca2 V3 102.37(5) 6 . ?
V1 Ca2 V3 107.22(5) 5_565 . ?
V2 Ca2 V3 104.95(4) 8_444 . ?
O2 Ca2 V1 29.42(12) 5_565 5_565 ?
O2 Ca2 V1 136.73(13) 5_565 6 ?
O2 Ca2 V2 152.23(12) 5_565 8_444 ?
O2 Ca2 V3 79.15(11) 5_565 . ?
O3 Ca2 V1 143.71(13) 6 5_565 ?
O3 Ca2 V1 32.10(12) 6 6 ?
O3 Ca2 V2 64.42(12) 6 8_444 ?
O3 Ca2 V3 74.00(12) 6 . ?
O3 Ca2 O2 140.69(18) 6 5_565 ?
O3 Ca2 O4 64.4(2) 6 6 ?
O3 Ca2 O10 96.83(18) 6 6 ?
O4 Ca2 V1 95.34(16) 6 5_565 ?
O4 Ca2 V1 97.75(17) 5_565 6 ?
O4 Ca2 V1 32.70(18) 6 6 ?
O4 Ca2 V1 27.98(18) 5_565 5_565 ?
O4 Ca2 V2 122.3(2) 5_565 8_444 ?
O4 Ca2 V2 75.41(19) 6 8_444 ?
O4 Ca2 V3 132.5(2) 5_565 . ?
O4 Ca2 V3 133.5(2) 6 . ?
O4 Ca2 O2 57.4(2) 5_565 5_565 ?
O4 Ca2 O2 122.1(2) 6 5_565 ?
O4 Ca2 O3 128.5(2) 5_565 6 ?
O4 Ca2 O4 68.9(3) 5_565 6 ?
O4 Ca2 O10 120.2(2) 5_565 6 ?
O5 Ca2 V1 73.13(15) 5_565 6 ?
O5 Ca2 V1 73.75(16) 5_565 5_565 ?
O5 Ca2 V2 138.61(16) 5_565 8_444 ?
O5 Ca2 V3 65.26(17) 5_565 . ?
O5 Ca2 O2 68.48(18) 5_565 5_565 ?
O5 Ca2 O3 74.37(19) 5_565 6 ?
O5 Ca2 O4 80.6(3) 5_565 5_565 ?
O5 Ca2 O4 83.9(3) 5_565 6 ?
O5 Ca2 O6 140.0(2) 5_565 8_444 ?
O5 Ca2 O10 76.7(2) 5_565 6 ?
O6 Ca2 V1 88.27(16) 8_444 6 ?
O6 Ca2 V1 144.19(16) 8_444 5_565 ?
O6 Ca2 V2 24.34(17) 8_444 8_444 ?
O6 Ca2 V3 85.56(18) 8_444 . ?
O6 Ca2 O2 134.5(2) 8_444 5_565 ?
O6 Ca2 O3 71.6(2) 8_444 6 ?
O6 Ca2 O4 99.4(2) 8_444 6 ?
O6 Ca2 O4 137.9(3) 8_444 5_565 ?
O6 Ca2 O10 87.2(3) 8_444 6 ?
O7 Ca2 V1 74.4(2) 10_564 5_565 ?
O7 Ca2 V1 143.1(2) 10_564 6 ?
O7 Ca2 V2 79.3(2) 10_564 8_444 ?
O7 Ca2 V3 105.1(2) 10_564 . ?
O7 Ca2 O2 73.2(2) 10_564 5_565 ?
O7 Ca2 O3 141.4(3) 10_564 6 ?
O7 Ca2 O4 120.1(3) 10_564 6 ?
O7 Ca2 O4 81.4(3) 10_564 5_565 ?
O7 Ca2 O5 141.6(3) 10_564 5_565 ?
O7 Ca2 O6 69.9(3) 10_564 8_444 ?
O7 Ca2 O10 83.7(3) 10_564 6 ?
O10 Ca2 V1 125.94(14) 6 6 ?
O10 Ca2 V1 92.29(16) 6 5_565 ?
O10 Ca2 V2 110.84(18) 6 8_444 ?
O10 Ca2 V3 23.57(13) 6 . ?
O10 Ca2 O2 62.9(2) 6 5_565 ?
O10 Ca2 O4 156.2(3) 6 6 ?
Ca4 Ca3 Ca5 107.99(18) . 16_554 ?
V2 Ca3 Ca4 61.05(3) . . ?
V2 Ca3 Ca4 60.49(3) 6_655 . ?
V2 Ca3 Ca5 106.6(2) 6_655 16_554 ?
V2 Ca3 Ca5 82.1(2) . 16_554 ?
V2 Ca3 V2 120.62(6) . 6_655 ?
O1 Ca3 Ca4 73.6(3) . . ?
O1 Ca3 Ca5 41.7(3) . 16_554 ?
O1 Ca3 V2 69.5(2) . 6_655 ?
O1 Ca3 V2 85.3(3) . . ?
O1 Ca3 O6 76.2(3) . . ?
O1 Ca3 O7 65.3(3) . 6_655 ?
O1 Ca3 O8 96.7(3) . . ?
O1 Ca3 O8 86.0(3) . 6_655 ?
O2 Ca3 Ca4 118.68(16) 14_544 . ?
O2 Ca3 Ca5 130.4(3) 14_544 16_554 ?
O2 Ca3 V2 134.4(2) 14_544 . ?
O2 Ca3 V2 83.95(16) 14_544 6_655 ?
O2 Ca3 O1 140.2(3) 14_544 . ?
O2 Ca3 O6 137.5(2) 14_544 . ?
O2 Ca3 O7 76.6(2) 14_544 6_655 ?
O2 Ca3 O8 85.1(2) 14_544 6_655 ?
O2 Ca3 O8 116.5(2) 14_544 . ?
O3 Ca3 Ca4 119.67(13) 15_554 . ?
O3 Ca3 Ca5 99.8(2) 15_554 16_554 ?
O3 Ca3 V2 71.69(13) 15_554 . ?
O3 Ca3 V2 151.95(13) 15_554 6_655 ?
O3 Ca3 O1 138.5(2) 15_554 . ?
O3 Ca3 O2 71.7(2) 15_554 14_544 ?
O3 Ca3 O6 66.13(19) 15_554 . ?
O3 Ca3 O7 144.4(2) 15_554 6_655 ?
O3 Ca3 O8 130.47(17) 15_554 6_655 ?
O3 Ca3 O8 81.33(19) 15_554 . ?
O3 Ca3 O10 82.9(2) 15_554 16_554 ?
O6 Ca3 Ca4 87.78(12) . . ?
O6 Ca3 Ca5 55.3(3) . 16_554 ?
O6 Ca3 V2 138.22(13) . 6_655 ?
O6 Ca3 V2 31.51(13) . . ?
O6 Ca3 O7 140.5(2) . 6_655 ?
O7 Ca3 Ca4 89.50(15) 6_655 . ?
O7 Ca3 Ca5 88.5(3) 6_655 16_554 ?
O7 Ca3 V2 30.84(15) 6_655 6_655 ?
O7 Ca3 V2 143.86(17) 6_655 . ?
O8 Ca3 Ca4 39.22(14) . . ?
O8 Ca3 Ca4 39.27(14) 6_655 . ?
O8 Ca3 Ca5 127.6(2) 6_655 16_554 ?
O8 Ca3 Ca5 109.8(3) . 16_554 ?
O8 Ca3 V2 31.22(13) . . ?
O8 Ca3 V2 30.20(13) 6_655 6_655 ?
O8 Ca3 V2 97.99(14) . 6_655 ?
O8 Ca3 V2 98.77(14) 6_655 . ?
O8 Ca3 O6 127.05(18) 6_655 . ?
O8 Ca3 O6 62.71(19) . . ?
O8 Ca3 O7 128.3(2) . 6_655 ?
O8 Ca3 O7 60.4(2) 6_655 6_655 ?
O8 Ca3 O8 70.7(3) . 6_655 ?
O10 Ca3 Ca4 154.82(19) 16_554 . ?
O10 Ca3 Ca5 53.4(2) 16_554 16_554 ?
O10 Ca3 V2 123.67(16) 16_554 . ?
O10 Ca3 V2 105.41(16) 16_554 6_655 ?
O10 Ca3 O1 81.9(3) 16_554 . ?
O10 Ca3 O2 77.1(2) 16_554 14_544 ?
O10 Ca3 O6 92.3(2) 16_554 . ?
O10 Ca3 O7 74.6(2) 16_554 6_655 ?
O10 Ca3 O8 154.3(2) 16_554 . ?
O10 Ca3 O8 134.3(2) 16_554 6_655 ?
V1 Ca4 V1 107.95(5) 6_655 . ?
V1 Ca4 V1 107.95(5) 6_655 5_665 ?
V1 Ca4 V1 107.95(5) 5_665 . ?
V2 Ca4 V1 70.29(3) . . ?
V2 Ca4 V1 72.39(3) . 5_665 ?
V2 Ca4 V1 178.17(7) 5_665 . ?
V2 Ca4 V1 178.17(7) . 6_655 ?
V2 Ca4 V1 72.39(3) 6_655 . ?
V2 Ca4 V1 70.29(3) 5_665 5_665 ?
V2 Ca4 V1 72.39(3) 5_665 6_655 ?
V2 Ca4 V1 178.17(7) 6_655 5_665 ?
V2 Ca4 V1 70.29(3) 6_655 6_655 ?
V2 Ca4 V2 109.35(5) 5_665 6_655 ?
V2 Ca4 V2 109.35(5) 6_655 . ?
V2 Ca4 V2 109.35(5) 5_665 . ?
O4 Ca4 V1 23.4(3) 6_655 6_655 ?
O4 Ca4 V1 23.4(3) . . ?
O4 Ca4 V1 91.7(2) 5_665 6_655 ?
O4 Ca4 V1 98.2(2) 5_665 . ?
O4 Ca4 V1 98.2(2) . 6_655 ?
O4 Ca4 V1 91.7(2) 6_655 . ?
O4 Ca4 V1 23.4(3) 5_665 5_665 ?
O4 Ca4 V1 98.2(2) 6_655 5_665 ?
O4 Ca4 V1 91.7(2) . 5_665 ?
O4 Ca4 V2 155.0(3) 6_655 . ?
O4 Ca4 V2 88.04(19) 5_665 . ?
O4 Ca4 V2 88.04(19) 6_655 5_665 ?
O4 Ca4 V2 80.0(2) . . ?
O4 Ca4 V2 155.0(3) . 5_665 ?
O4 Ca4 V2 80.0(2) 5_665 5_665 ?
O4 Ca4 V2 88.04(19) . 6_655 ?
O4 Ca4 V2 80.0(2) 6_655 6_655 ?
O4 Ca4 V2 155.0(3) 5_665 6_655 ?
O4 Ca4 O4 77.2(4) 5_665 6_655 ?
O4 Ca4 O4 77.2(4) 5_665 . ?
O4 Ca4 O4 77.2(4) 6_655 . ?
O4 Ca4 O8 106.5(3) 5_665 . ?
O4 Ca4 O8 100.8(3) 5_665 5_665 ?
O4 Ca4 O8 175.4(3) . 5_665 ?
O4 Ca4 O8 175.4(3) 6_655 . ?
O4 Ca4 O8 106.5(3) 6_655 5_665 ?
O4 Ca4 O8 175.4(3) 5_665 6_655 ?
O4 Ca4 O8 100.8(3) . . ?
O4 Ca4 O8 100.8(3) 6_655 6_655 ?
O4 Ca4 O8 106.5(3) . 6_655 ?
O8 Ca4 V1 156.14(15) . 6_655 ?
O8 Ca4 V1 85.87(13) 6_655 . ?
O8 Ca4 V1 85.03(13) 6_655 6_655 ?
O8 Ca4 V1 85.87(13) 5_665 6_655 ?
O8 Ca4 V1 85.03(12) . . ?
O8 Ca4 V1 85.87(13) . 5_665 ?
O8 Ca4 V1 156.14(15) 5_665 . ?
O8 Ca4 V1 85.03(13) 5_665 5_665 ?
O8 Ca4 V1 156.14(15) 6_655 5_665 ?
O8 Ca4 V2 95.29(14) 5_665 6_655 ?
O8 Ca4 V2 25.22(13) . . ?
O8 Ca4 V2 25.22(13) 5_665 5_665 ?
O8 Ca4 V2 25.22(13) 6_655 6_655 ?
O8 Ca4 V2 95.96(14) 6_655 5_665 ?
O8 Ca4 V2 95.96(14) . 6_655 ?
O8 Ca4 V2 95.96(14) 5_665 . ?
O8 Ca4 V2 95.29(14) . 5_665 ?
O8 Ca4 V2 95.29(14) 6_655 . ?
O8 Ca4 O8 75.8(2) 5_665 6_655 ?
O8 Ca4 O8 75.8(2) 5_665 . ?
O8 Ca4 O8 75.8(2) 6_655 . ?
Ca1 Ca5 V1 56.3(2) 8_444 8_444 ?
Ca5 Ca5 Ca1 123.6(10) 5 8_444 ?
Ca5 Ca5 Ca1 157.7(4) 6 8_444 ?
Ca5 Ca5 Ca5 60.002(8) 5 6 ?
Ca5 Ca5 V1 116.2(7) 6 8_444 ?
Ca5 Ca5 V1 91.8(9) 6 10_554 ?
Ca5 Ca5 V1 68.8(7) 5 8_444 ?
Ca5 Ca5 V1 133.0(5) 5 10_554 ?
Ca5 Ca5 V3 79.0(3) 5 . ?
Ca5 Ca5 V3 79.0(3) 6 . ?
Ca5 Ca5 O1 79.9(11) 6 10_554 ?
Ca5 Ca5 O1 138.4(11) 5 10_554 ?
Ca5 Ca5 O1 72.8(10) 5 8_444 ?
Ca5 Ca5 O1 131.5(10) 6 8_444 ?
Ca5 Ca5 O2 124.5(3) 5 10_554 ?
Ca5 Ca5 O2 113.3(6) 6 10_554 ?
Ca5 Ca5 O6 149.2(10) 5 10_554 ?
Ca5 Ca5 O6 144.8(10) 6 10_554 ?
Ca5 Ca5 O10 110.0(3) 6 5 ?
Ca5 Ca5 O10 83.7(6) 5 5 ?
Ca5 Ca5 O10 73.0(6) 6 . ?
Ca5 Ca5 O10 103.6(5) 5 . ?
V1 Ca5 Ca1 70.0(3) 10_554 8_444 ?
V1 Ca5 V1 97.1(3) 10_554 8_444 ?
V3 Ca5 Ca1 122.9(5) . 8_444 ?
V3 Ca5 V1 126.2(3) . 8_444 ?
V3 Ca5 V1 135.5(4) . 10_554 ?
V3 Ca5 O2 156.4(5) . 10_554 ?
V3 Ca5 O6 88.3(4) . 10_554 ?
O1 Ca5 Ca1 89.3(5) 10_554 8_444 ?
O1 Ca5 Ca1 52.6(3) 8_444 8_444 ?
O1 Ca5 V1 26.8(2) 8_444 8_444 ?
O1 Ca5 V1 127.4(5) 10_554 8_444 ?
O1 Ca5 V1 30.4(2) 10_554 10_554 ?
O1 Ca5 V1 114.4(5) 8_444 10_554 ?
O1 Ca5 V3 105.4(4) 10_554 . ?
O1 Ca5 V3 103.5(4) 8_444 . ?
O1 Ca5 O1 140.9(6) 10_554 8_444 ?
O1 Ca5 O2 59.9(3) 10_554 10_554 ?
O1 Ca5 O2 83.7(4) 8_444 10_554 ?
O1 Ca5 O6 71.9(5) 10_554 10_554 ?
O1 Ca5 O6 83.3(5) 8_444 10_554 ?
O1 Ca5 O10 123.2(5) 10_554 5 ?
O1 Ca5 O10 73.0(4) 8_444 5 ?
O1 Ca5 O10 132.5(5) 8_444 . ?
O1 Ca5 O10 72.1(4) 10_554 . ?
O2 Ca5 Ca1 45.0(2) 10_554 8_444 ?
O2 Ca5 V1 30.78(15) 10_554 10_554 ?
O2 Ca5 V1 68.1(3) 10_554 8_444 ?
O6 Ca5 Ca1 44.0(2) 10_554 8_444 ?
O6 Ca5 V1 97.9(4) 10_554 8_444 ?
O6 Ca5 V1 74.5(3) 10_554 10_554 ?
O6 Ca5 O2 70.0(3) 10_554 10_554 ?
O10 Ca5 Ca1 122.2(5) . 8_444 ?
O10 Ca5 Ca1 92.3(4) 5 8_444 ?
O10 Ca5 V1 102.2(3) . 10_554 ?
O10 Ca5 V1 143.3(5) 5 10_554 ?
O10 Ca5 V1 99.0(3) 5 8_444 ?
O10 Ca5 V1 158.5(4) . 8_444 ?
O10 Ca5 V3 33.37(16) . . ?
O10 Ca5 V3 33.79(17) 5 . ?
O10 Ca5 O2 136.2(6) 5 10_554 ?
O10 Ca5 O2 128.3(4) . 10_554 ?
O10 Ca5 O6 70.8(4) 5 10_554 ?
O10 Ca5 O6 78.4(4) . 10_554 ?
O10 Ca5 O10 59.6(3) 5 . ?
Ca1 V1 Ca1 133.96(8) . 6_665 ?
Ca1 V1 Ca2 157.16(6) . 6_665 ?
Ca1 V1 Ca4 103.09(5) . . ?
Ca1 V1 Ca5 59.2(3) . 14_554 ?
Ca1 V1 Ca5 78.1(3) . 16_554 ?
Ca2 V1 Ca1 151.82(6) 5 6_665 ?
Ca2 V1 Ca1 68.52(5) 6_665 6_665 ?
Ca2 V1 Ca1 74.09(5) 5 . ?
Ca2 V1 Ca2 83.31(6) 5 6_665 ?
Ca2 V1 Ca4 66.25(5) 5 . ?
Ca2 V1 Ca4 63.71(4) 6_665 . ?
Ca2 V1 Ca5 151.9(3) 5 16_554 ?
Ca2 V1 Ca5 133.3(3) 5 14_554 ?
Ca2 V1 Ca5 143.3(3) 6_665 14_554 ?
Ca4 V1 Ca1 98.99(4) . 6_665 ?
Ca5 V1 Ca1 55.9(3) 16_554 6_665 ?
Ca5 V1 Ca1 74.8(3) 14_554 6_665 ?
Ca5 V1 Ca2 124.0(3) 16_554 6_665 ?
Ca5 V1 Ca4 117.0(2) 16_554 . ?
Ca5 V1 Ca4 122.24(19) 14_554 . ?
Ca5 V1 Ca5 19.4(5) 16_554 14_554 ?
O1 V1 Ca1 56.4(4) . . ?
O1 V1 Ca1 88.1(3) . 6_665 ?
O1 V1 Ca2 111.9(3) . 5 ?
O1 V1 Ca2 133.1(4) . 6_665 ?
O1 V1 Ca4 81.7(4) . . ?
O1 V1 Ca5 41.4(4) . 14_554 ?
O1 V1 Ca5 46.1(4) . 16_554 ?
O1 V1 O2 114.8(4) . . ?
O1 V1 O3 103.8(4) . . ?
O1 V1 O4 113.0(5) . . ?
O1 V1 Ca5A 54(4) . 14_554 ?
O2 V1 Ca1 31.9(2) . 6_665 ?
O2 V1 Ca1 136.6(3) . . ?
O2 V1 Ca2 133.3(3) . 5 ?
O2 V1 Ca2 63.4(3) . 6_665 ?
O2 V1 Ca4 118.3(3) . . ?
O2 V1 Ca5 86.3(4) . 14_554 ?
O2 V1 Ca5 72.0(3) . 16_554 ?
O2 V1 O3 118.5(3) . . ?
O2 V1 O4 104.8(4) . . ?
O2 V1 Ca5A 72.0(19) . 14_554 ?
O3 V1 Ca1 147.05(17) . 6_665 ?
O3 V1 Ca1 47.42(17) . . ?
O3 V1 Ca2 118.05(17) . 6_665 ?
O3 V1 Ca2 49.46(16) . 5 ?
O3 V1 Ca4 112.93(16) . . ?
O3 V1 Ca5 112.0(3) . 16_554 ?
O3 V1 Ca5 93.9(3) . 14_554 ?
O3 V1 O4 101.4(3) . . ?
O3 V1 Ca5A 98.0(19) . 14_554 ?
O4 V1 Ca1 101.8(3) . 6_665 ?
O4 V1 Ca1 117.9(2) . . ?
O4 V1 Ca2 52.8(3) . 5 ?
O4 V1 Ca2 41.5(2) . 6_665 ?
O4 V1 Ca4 31.4(3) . . ?
O4 V1 Ca5 143.6(4) . 16_554 ?
O4 V1 Ca5 153.5(4) . 14_554 ?
O4 V1 Ca5A 159(3) . 14_554 ?
Ca5A V1 Ca1 70.9(6) 14_554 . ?
Ca5A V1 Ca4 131(4) 14_554 . ?
Ca5A V1 Ca5 16(3) 14_554 16_554 ?
Ca1 V2 Ca1 86.47(8) 6_665 5_665 ?
Ca1 V2 Ca2 120.26(5) 5_665 14_554 ?
Ca1 V2 Ca2 74.21(5) 6_665 14_554 ?
Ca1 V2 Ca3 85.07(5) 5_665 5_665 ?
Ca1 V2 Ca3 99.93(5) 6_665 . ?
Ca1 V2 Ca3 170.92(6) 6_665 5_665 ?
Ca1 V2 Ca4 103.72(5) 5_665 . ?
Ca1 V2 Ca4 115.23(6) 6_665 . ?
Ca3 V2 Ca1 168.11(6) . 5_665 ?
Ca3 V2 Ca2 71.37(4) . 14_554 ?
Ca3 V2 Ca2 113.08(5) 5_665 14_554 ?
Ca3 V2 Ca3 87.84(6) . 5_665 ?
Ca3 V2 Ca4 63.86(4) 5_665 . ?
Ca3 V2 Ca4 64.51(4) . . ?
Ca4 V2 Ca2 135.80(5) . 14_554 ?
O5 V2 Ca1 59.9(2) . 6_665 ?
O5 V2 Ca1 51.4(2) . 5_665 ?
O5 V2 Ca2 133.0(2) . 14_554 ?
O5 V2 Ca3 111.8(2) . 5_665 ?
O5 V2 Ca3 123.7(3) . . ?
O5 V2 Ca4 77.7(3) . . ?
O5 V2 O6 107.1(3) . . ?
O5 V2 O7 104.7(4) . . ?
O5 V2 O8 112.2(3) . . ?
O6 V2 Ca1 129.7(2) . 5_665 ?
O6 V2 Ca1 49.6(2) . 6_665 ?
O6 V2 Ca2 36.1(2) . 14_554 ?
O6 V2 Ca3 139.5(2) . 5_665 ?
O6 V2 Ca3 60.8(2) . . ?
O6 V2 Ca4 115.7(3) . . ?
O6 V2 O8 108.2(3) . . ?
O7 V2 Ca1 116.3(3) . 6_665 ?
O7 V2 Ca1 53.3(3) . 5_665 ?
O7 V2 Ca2 85.8(3) . 14_554 ?
O7 V2 Ca3 60.5(3) . 5_665 ?
O7 V2 Ca3 129.9(3) . . ?
O7 V2 Ca4 120.6(3) . . ?
O7 V2 O6 119.5(4) . . ?
O7 V2 O8 105.2(3) . . ?
O8 V2 Ca1 138.51(18) . 6_665 ?
O8 V2 Ca1 121.89(18) . 5_665 ?
O8 V2 Ca2 108.56(19) . 14_554 ?
O8 V2 Ca3 45.98(17) . 5_665 ?
O8 V2 Ca3 47.47(17) . . ?
O8 V2 Ca4 34.90(19) . . ?
Ca1 V3 Ca1 82.25(6) 5 6 ?
Ca1 V3 Ca1 82.25(6) 5 . ?
Ca1 V3 Ca1 82.25(6) 6 . ?
Ca1 V3 Ca2 66.78(3) 5 6 ?
Ca1 V3 Ca2 71.04(4) 6 6 ?
Ca1 V3 Ca2 141.03(7) 6 5 ?
Ca1 V3 Ca2 66.78(3) . 5 ?
Ca1 V3 Ca2 141.03(7) . 6 ?
Ca1 V3 Ca2 71.04(4) 5 5 ?
Ca2 V3 Ca2 119.913(4) 6 5 ?
Ca5 V3 Ca1 127.4(2) 5 . ?
Ca5 V3 Ca1 142.3(3) . . ?
Ca5 V3 Ca1 142.3(3) 6 6 ?
Ca5 V3 Ca1 120.4(3) . 5 ?
Ca5 V3 Ca1 120.4(3) 6 . ?
Ca5 V3 Ca1 120.4(3) 5 6 ?
Ca5 V3 Ca1 127.3(2) 6 5 ?
Ca5 V3 Ca1 127.3(2) . 6 ?
Ca5 V3 Ca1 142.3(3) 5 5 ?
Ca5 V3 Ca2 76.2(3) . 6 ?
Ca5 V3 Ca2 97.6(2) 6 6 ?
Ca5 V3 Ca2 91.1(2) 5 6 ?
Ca5 V3 Ca2 91.1(2) . 5 ?
Ca5 V3 Ca2 76.2(3) 6 5 ?
Ca5 V3 Ca2 97.6(2) 5 5 ?
Ca5 V3 Ca5 22.0(5) . 5 ?
Ca5 V3 Ca5 22.0(5) 5 6 ?
Ca5 V3 Ca5 22.0(5) . 6 ?
O9 V3 Ca1 49.41(4) . . ?
O9 V3 Ca1 49.41(4) . 5 ?
O9 V3 Ca1 49.41(4) . 6 ?
O9 V3 Ca2 91.71(4) . 5 ?
O9 V3 Ca2 91.71(4) . 6 ?
O9 V3 Ca5 167.3(3) . 5 ?
O9 V3 Ca5 167.3(3) . . ?
O9 V3 Ca5 167.3(3) . 6 ?
O9 V3 O10 106.8(3) . . ?
O9 V3 O10 106.8(3) . 5 ?
O9 V3 O10 106.8(3) . 6 ?
O10 V3 Ca1 100.9(2) 6 6 ?
O10 V3 Ca1 144.8(3) 5 . ?
O10 V3 Ca1 100.9(2) . . ?
O10 V3 Ca1 144.8(3) . 6 ?
O10 V3 Ca1 63.8(3) 6 . ?
O10 V3 Ca1 100.9(2) 5 5 ?
O10 V3 Ca1 63.8(3) 5 6 ?
O10 V3 Ca1 144.8(3) 6 5 ?
O10 V3 Ca1 63.8(3) . 5 ?
O10 V3 Ca2 86.5(2) . 6 ?
O10 V3 Ca2 147.7(2) 6 6 ?
O10 V3 Ca2 35.9(2) . 5 ?
O10 V3 Ca2 147.7(2) 5 5 ?
O10 V3 Ca2 86.5(2) 6 5 ?
O10 V3 Ca2 35.9(2) 5 6 ?
O10 V3 Ca5 85.8(4) . 5 ?
O10 V3 Ca5 85.8(4) 5 6 ?
O10 V3 Ca5 69.2(3) 5 5 ?
O10 V3 Ca5 65.4(4) 5 . ?
O10 V3 Ca5 69.2(3) 6 6 ?
O10 V3 Ca5 85.8(4) 6 . ?
O10 V3 Ca5 65.4(4) 6 5 ?
O10 V3 Ca5 69.2(3) . . ?
O10 V3 Ca5 65.4(4) . 6 ?
O10 V3 O10 112.0(2) 5 6 ?
O10 V3 O10 112.0(2) 6 . ?
O10 V3 O10 112.0(2) 5 . ?
Ca3 O1 Ca1 121.3(4) . . ?
Ca3 O1 Ca5 104.6(4) . 14_554 ?
Ca3 O1 Ca5A 114(5) . 14_554 ?
Ca5 O1 Ca1 106.3(6) 16_554 . ?
Ca5 O1 Ca1 79.9(5) 14_554 . ?
Ca5 O1 Ca3 96.4(4) 16_554 . ?
Ca5 O1 Ca5 27.3(7) 16_554 14_554 ?
Ca5 O1 Ca5A 19(4) 16_554 14_554 ?
Ca5 O1 Ca5A 19(3) 14_554 14_554 ?
V1 O1 Ca1 91.9(3) . . ?
V1 O1 Ca3 134.5(7) . . ?
V1 O1 Ca5 103.5(5) . 16_554 ?
V1 O1 Ca5 111.8(6) . 14_554 ?
V1 O1 Ca5A 95(5) . 14_554 ?
Ca5A O1 Ca1 89.6(15) 14_554 . ?
Ca1 O2 Ca2 93.1(2) 6_665 6_665 ?
Ca1 O2 Ca5 70.6(3) 6_665 16_554 ?
Ca1 O2 Ca5A 82(2) 6_665 14_554 ?
Ca2 O2 Ca5 142.1(3) 6_665 16_554 ?
Ca3 O2 Ca1 96.7(2) 8_554 6_665 ?
Ca3 O2 Ca2 83.3(2) 8_554 6_665 ?
Ca3 O2 Ca5 131.1(4) 8_554 16_554 ?
Ca3 O2 Ca5A 120(3) 8_554 14_554 ?
V1 O2 Ca1 126.9(3) . 6_665 ?
V1 O2 Ca2 87.2(3) . 6_665 ?
V1 O2 Ca3 135.9(3) . 8_554 ?
V1 O2 Ca5 77.2(3) . 16_554 ?
V1 O2 Ca5A 77.5(8) . 14_554 ?
Ca5A O2 Ca5 16(3) 14_554 16_554 ?
Ca1 O3 Ca2 105.08(19) . 5 ?
Ca3 O3 Ca1 99.84(19) 9_454 . ?
Ca3 O3 Ca2 111.6(2) 9_454 5 ?
V1 O3 Ca1 100.8(2) . . ?
V1 O3 Ca2 98.4(2) . 5 ?
V1 O3 Ca3 137.3(3) . 9_454 ?
Ca2 O4 Ca2 124.6(4) 6_665 5 ?
Ca4 O4 Ca2 103.5(3) . 6_665 ?
Ca4 O4 Ca2 100.2(3) . 5 ?
V1 O4 Ca2 110.5(3) . 6_665 ?
V1 O4 Ca2 94.5(3) . 5 ?
V1 O4 Ca4 125.1(5) . . ?
Ca1 O5 Ca1 112.0(3) 5_665 6_665 ?
Ca2 O5 Ca1 102.2(2) 6_665 5_665 ?
Ca2 O5 Ca1 106.5(2) 6_665 6_665 ?
V2 O5 Ca1 87.4(2) . 6_665 ?
V2 O5 Ca1 97.9(3) . 5_665 ?
V2 O5 Ca2 148.9(4) . 6_665 ?
Ca1 O6 Ca2 114.6(3) 6_665 14_554 ?
Ca1 O6 Ca3 137.2(3) 6_665 . ?
Ca1 O6 Ca5 73.8(3) 6_665 16_554 ?
Ca2 O6 Ca3 98.4(2) 14_554 . ?
Ca2 O6 Ca5 98.3(3) 14_554 16_554 ?
Ca3 O6 Ca5 75.3(3) . 16_554 ?
V2 O6 Ca1 97.9(3) . 6_665 ?
V2 O6 Ca2 119.6(4) . 14_554 ?
V2 O6 Ca3 87.7(2) . . ?
V2 O6 Ca5 140.5(4) . 16_554 ?
Ca1 O7 Ca3 107.4(3) 5_665 5_665 ?
Ca2 O7 Ca1 110.0(3) 16_654 5_665 ?
Ca2 O7 Ca3 90.2(3) 16_654 5_665 ?
V2 O7 Ca1 95.7(3) . 5_665 ?
V2 O7 Ca2 153.3(5) . 16_654 ?
V2 O7 Ca3 88.6(3) . 5_665 ?
Ca3 O8 Ca3 136.8(2) . 5_665 ?
Ca4 O8 Ca3 98.8(2) . . ?
Ca4 O8 Ca3 98.37(19) . 5_665 ?
V2 O8 Ca3 103.8(2) . 5_665 ?
V2 O8 Ca3 101.3(2) . . ?
V2 O8 Ca4 119.9(3) . . ?
Ca1 O9 Ca1 116.56(16) 5 . ?
Ca1 O9 Ca1 116.56(16) 6 5 ?
Ca1 O9 Ca1 116.56(16) 6 . ?
V3 O9 Ca1 100.8(2) . 5 ?
V3 O9 Ca1 100.8(2) . 6 ?
V3 O9 Ca1 100.8(2) . . ?
Ca2 O10 Ca1 95.4(2) 5 5 ?
Ca2 O10 Ca5 125.6(4) 5 . ?
Ca2 O10 Ca5 103.7(4) 5 6 ?
Ca3 O10 Ca1 84.5(2) 10_554 5 ?
Ca3 O10 Ca2 98.30(19) 10_554 5 ?
Ca3 O10 Ca5 97.1(3) 10_554 6 ?
Ca3 O10 Ca5 85.5(3) 10_554 . ?
Ca5 O10 Ca1 160.3(4) 6 5 ?
Ca5 O10 Ca1 138.9(4) . 5 ?
Ca5 O10 Ca5 23.3(6) 6 . ?
V3 O10 Ca1 85.6(3) . 5 ?
V3 O10 Ca2 120.5(3) . 5 ?
V3 O10 Ca3 140.6(3) . 10_554 ?
V3 O10 Ca5 80.8(4) . 6 ?
V3 O10 Ca5 77.5(3) . . ?
Ca1 Ca5A Ca1 117(2) 10_554 8_444 ?
V1 Ca5A Ca1 53.8(11) 8_444 8_444 ?
V1 Ca5A Ca1 143(7) 8_444 10_554 ?
V1 Ca5A Ca1 64.3(14) 9_454 10_554 ?
V1 Ca5A Ca1 53.8(11) 10_554 10_554 ?
V1 Ca5A Ca1 64.3(14) 10_554 8_444 ?
V1 Ca5A Ca1 143(7) 9_454 8_444 ?
V1 Ca5A V1 101(5) 9_454 10_554 ?
V1 Ca5A V1 101(5) 8_444 10_554 ?
V1 Ca5A V1 101(5) 8_444 9_454 ?
V1 Ca5A V3 117(4) 8_444 . ?
V1 Ca5A V3 117(4) 10_554 . ?
V1 Ca5A V3 117(4) 9_454 . ?
V3 Ca5A Ca1 100(4) . 8_444 ?
V3 Ca5A Ca1 100(4) . 10_554 ?
O1 Ca5A Ca1 76.6(7) 9_454 10_554 ?
O1 Ca5A Ca1 162(4) 9_454 8_444 ?
O1 Ca5A Ca1 76.6(7) 10_554 8_444 ?
O1 Ca5A Ca1 45.4(6) 8_444 8_444 ?
O1 Ca5A Ca1 162(4) 8_444 10_554 ?
O1 Ca5A Ca1 45.4(6) 10_554 10_554 ?
O1 Ca5A V1 30.9(14) 8_444 8_444 ?
O1 Ca5A V1 126(4) 8_444 9_454 ?
O1 Ca5A V1 30.9(14) 10_554 10_554 ?
O1 Ca5A V1 126(4) 10_554 8_444 ?
O1 Ca5A V1 30.9(14) 9_454 9_454 ?
O1 Ca5A V1 109(3) 9_454 8_444 ?
O1 Ca5A V1 109(3) 8_444 10_554 ?
O1 Ca5A V1 126(4) 9_454 10_554 ?
O1 Ca5A V1 109(3) 10_554 9_454 ?
O1 Ca5A V3 88(5) 10_554 . ?
O1 Ca5A V3 88(5) 8_444 . ?
O1 Ca5A V3 88(5) 9_454 . ?
O1 Ca5A O1 119.9(7) 10_554 9_454 ?
O1 Ca5A O1 119.9(7) 8_444 9_454 ?
O1 Ca5A O1 119.9(7) 10_554 8_444 ?
O1 Ca5A O2 58(2) 9_454 9_454 ?
O1 Ca5A O2 81(3) 9_454 8_444 ?
O1 Ca5A O2 81(3) 8_444 10_554 ?
O1 Ca5A O2 141(8) 10_554 8_444 ?
O1 Ca5A O2 141(8) 9_454 10_554 ?
O1 Ca5A O2 58(2) 8_444 8_444 ?
O1 Ca5A O2 58(2) 10_554 10_554 ?
O1 Ca5A O2 141(8) 8_444 9_454 ?
O1 Ca5A O2 81(3) 10_554 9_454 ?
O2 Ca5A Ca1 40.9(8) 9_454 10_554 ?
O2 Ca5A Ca1 82(3) 10_554 10_554 ?
O2 Ca5A Ca1 82(3) 8_444 8_444 ?
O2 Ca5A Ca1 40.9(8) 10_554 8_444 ?
O2 Ca5A Ca1 125(6) 9_454 8_444 ?
O2 Ca5A Ca1 125(6) 8_444 10_554 ?
O2 Ca5A V1 30.5(12) 9_454 9_454 ?
O2 Ca5A V1 30.5(12) 8_444 8_444 ?
O2 Ca5A V1 110(6) 8_444 10_554 ?
O2 Ca5A V1 70(3) 8_444 9_454 ?
O2 Ca5A V1 70(3) 9_454 10_554 ?
O2 Ca5A V1 70(3) 10_554 8_444 ?
O2 Ca5A V1 30.5(12) 10_554 10_554 ?
O2 Ca5A V1 110(6) 10_554 9_454 ?
O2 Ca5A V1 110(6) 9_454 8_444 ?
O2 Ca5A V3 129(3) 9_454 . ?
O2 Ca5A V3 129(3) 10_554 . ?
O2 Ca5A V3 129(3) 8_444 . ?
O2 Ca5A O2 85(5) 10_554 8_444 ?
O2 Ca5A O2 85(5) 10_554 9_454 ?
O2 Ca5A O2 85(5) 9_454 8_444 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Ca1 V1 O1 Ca1 148.8(3) 6_665 . . . ?
Ca1 V1 O1 Ca3 139.5(8) . . . . ?
Ca1 V1 O1 Ca3 -71.7(6) 6_665 . . . ?
Ca1 V1 O1 Ca5 41.6(5) 6_665 . . 16_554 ?
Ca1 V1 O1 Ca5 -107.2(7) . . . 16_554 ?
Ca1 V1 O1 Ca5 -79.9(6) . . . 14_554 ?
Ca1 V1 O1 Ca5 68.9(5) 6_665 . . 14_554 ?
Ca1 V1 O1 Ca5A 59.1(16) 6_665 . . 14_554 ?
Ca1 V1 O1 Ca5A -89.8(16) . . . 14_554 ?
Ca1 V1 O2 Ca1 102.3(4) . . . 6_665 ?
Ca1 V1 O2 Ca2 91.8(5) 6_665 . . 6_665 ?
Ca1 V1 O2 Ca2 -165.93(17) . . . 6_665 ?
Ca1 V1 O2 Ca3 169.2(10) 6_665 . . 8_554 ?
Ca1 V1 O2 Ca3 -88.5(7) . . . 8_554 ?
Ca1 V1 O2 Ca5 -53.5(5) 6_665 . . 16_554 ?
Ca1 V1 O2 Ca5 48.8(4) . . . 16_554 ?
Ca1 V1 O2 Ca5A -70(3) 6_665 . . 14_554 ?
Ca1 V1 O2 Ca5A 33(3) . . . 14_554 ?
Ca1 V1 O3 Ca1 -108.4(3) 6_665 . . . ?
Ca1 V1 O3 Ca2 144.4(2) 6_665 . . 5 ?
Ca1 V1 O3 Ca2 -107.2(2) . . . 5 ?
Ca1 V1 O3 Ca3 9.2(6) 6_665 . . 9_454 ?
Ca1 V1 O3 Ca3 117.6(4) . . . 9_454 ?
Ca1 V1 O4 Ca2 -166.30(17) 6_665 . . 5 ?
Ca1 V1 O4 Ca2 167.3(2) . . . 6_665 ?
Ca1 V1 O4 Ca2 37.8(4) . . . 5 ?
Ca1 V1 O4 Ca2 -36.7(4) 6_665 . . 6_665 ?
Ca1 V1 O4 Ca4 87.9(4) 6_665 . . . ?
Ca1 V1 O4 Ca4 -68.0(5) . . . . ?
Ca1 V2 O5 Ca1 111.9(3) 6_665 . . 5_665 ?
Ca1 V2 O5 Ca1 -111.9(3) 5_665 . . 6_665 ?
Ca1 V2 O5 Ca2 -118.3(7) 6_665 . . 6_665 ?
Ca1 V2 O5 Ca2 129.9(7) 5_665 . . 6_665 ?
Ca1 V2 O6 Ca1 35.7(4) 5_665 . . 6_665 ?
Ca1 V2 O6 Ca2 -88.5(3) 5_665 . . 14_554 ?
Ca1 V2 O6 Ca2 -124.2(5) 6_665 . . 14_554 ?
Ca1 V2 O6 Ca3 137.4(3) 6_665 . . . ?
Ca1 V2 O6 Ca3 173.12(11) 5_665 . . . ?
Ca1 V2 O6 Ca5 74.1(5) 6_665 . . 16_554 ?
Ca1 V2 O6 Ca5 109.8(6) 5_665 . . 16_554 ?
Ca1 V2 O7 Ca1 -63.1(3) 6_665 . . 5_665 ?
Ca1 V2 O7 Ca2 165.1(13) 5_665 . . 16_654 ?
Ca1 V2 O7 Ca2 102.0(10) 6_665 . . 16_654 ?
Ca1 V2 O7 Ca3 -107.3(3) 5_665 . . 5_665 ?
Ca1 V2 O7 Ca3 -170.38(8) 6_665 . . 5_665 ?
Ca1 V2 O8 Ca3 -46.9(4) 6_665 . . . ?
Ca1 V2 O8 Ca3 168.56(11) 6_665 . . 5_665 ?
Ca1 V2 O8 Ca3 -173.30(9) 5_665 . . . ?
Ca1 V2 O8 Ca3 42.1(3) 5_665 . . 5_665 ?
Ca1 V2 O8 Ca4 60.2(4) 6_665 . . . ?
Ca1 V2 O8 Ca4 -66.2(3) 5_665 . . . ?
Ca1 V3 O9 Ca1 -120.0(1) . . . 5 ?
Ca1 V3 O9 Ca1 -120.0(1) 6 . . . ?
Ca1 V3 O9 Ca1 120.0(2) 5 . . . ?
Ca1 V3 O9 Ca1 -120.0(1) 5 . . 6 ?
Ca1 V3 O9 Ca1 120.0(1) 6 . . 5 ?
Ca1 V3 O9 Ca1 120.0(1) . . . 6 ?
Ca1 V3 O10 Ca1 -16.4(4) 6 . . 5 ?
Ca1 V3 O10 Ca1 75.62(14) . . . 5 ?
Ca1 V3 O10 Ca2 -18.0(4) . . . 5 ?
Ca1 V3 O10 Ca2 -93.6(4) 5 . . 5 ?
Ca1 V3 O10 Ca2 -110.0(4) 6 . . 5 ?
Ca1 V3 O10 Ca3 75.8(6) 5 . . 10_554 ?
Ca1 V3 O10 Ca3 59.4(8) 6 . . 10_554 ?
Ca1 V3 O10 Ca3 151.4(6) . . . 10_554 ?
Ca1 V3 O10 Ca5 -142.1(3) . . . . ?
Ca1 V3 O10 Ca5 149.4(4) 6 . . 6 ?
Ca1 V3 O10 Ca5 165.8(3) 5 . . 6 ?
Ca1 V3 O10 Ca5 -118.6(3) . . . 6 ?
Ca1 V3 O10 Ca5 142.3(4) 5 . . . ?
Ca1 V3 O10 Ca5 125.9(4) 6 . . . ?
Ca2 V1 O1 Ca1 -153.34(17) 6_665 . . . ?
Ca2 V1 O1 Ca1 -51.6(4) 5 . . . ?
Ca2 V1 O1 Ca3 -13.9(9) 6_665 . . . ?
Ca2 V1 O1 Ca3 87.9(6) 5 . . . ?
Ca2 V1 O1 Ca5 -131.5(5) 5 . . 14_554 ?
Ca2 V1 O1 Ca5 126.8(5) 6_665 . . 14_554 ?
Ca2 V1 O1 Ca5 99.4(6) 6_665 . . 16_554 ?
Ca2 V1 O1 Ca5 -158.8(4) 5 . . 16_554 ?
Ca2 V1 O1 Ca5A 116.9(16) 6_665 . . 14_554 ?
Ca2 V1 O1 Ca5A -141.4(16) 5 . . 14_554 ?
Ca2 V1 O2 Ca1 -91.8(5) 6_665 . . 6_665 ?
Ca2 V1 O2 Ca1 -141.1(3) 5 . . 6_665 ?
Ca2 V1 O2 Ca2 -49.3(3) 5 . . 6_665 ?
Ca2 V1 O2 Ca3 77.5(6) 6_665 . . 8_554 ?
Ca2 V1 O2 Ca3 28.1(8) 5 . . 8_554 ?
Ca2 V1 O2 Ca5 165.4(3) 5 . . 16_554 ?
Ca2 V1 O2 Ca5 -145.2(3) 6_665 . . 16_554 ?
Ca2 V1 O2 Ca5A 149(3) 5 . . 14_554 ?
Ca2 V1 O2 Ca5A -162(3) 6_665 . . 14_554 ?
Ca2 V1 O3 Ca1 107.2(2) 5 . . . ?
Ca2 V1 O3 Ca1 158.22(9) 6_665 . . . ?
Ca2 V1 O3 Ca2 51.0(2) 6_665 . . 5 ?
Ca2 V1 O3 Ca3 -84.1(4) 6_665 . . 9_454 ?
Ca2 V1 O3 Ca3 -135.1(5) 5 . . 9_454 ?
Ca2 V1 O4 Ca2 -129.6(6) 6_665 . . 5 ?
Ca2 V1 O4 Ca2 129.6(6) 5 . . 6_665 ?
Ca2 V1 O4 Ca4 -105.8(5) 5 . . . ?
Ca2 V1 O4 Ca4 124.6(7) 6_665 . . . ?
Ca2 V2 O5 Ca1 -14.0(4) 14_554 . . 6_665 ?
Ca2 V2 O5 Ca1 97.9(2) 14_554 . . 5_665 ?
Ca2 V2 O5 Ca2 -132.2(5) 14_554 . . 6_665 ?
Ca2 V2 O6 Ca1 124.2(5) 14_554 . . 6_665 ?
Ca2 V2 O6 Ca3 -98.4(3) 14_554 . . . ?
Ca2 V2 O6 Ca5 -161.7(8) 14_554 . . 16_554 ?
Ca2 V2 O7 Ca1 -133.2(2) 14_554 . . 5_665 ?
Ca2 V2 O7 Ca2 31.9(10) 14_554 . . 16_654 ?
Ca2 V2 O7 Ca3 119.52(19) 14_554 . . 5_665 ?
Ca2 V2 O8 Ca3 -104.52(18) 14_554 . . 5_665 ?
Ca2 V2 O8 Ca3 40.1(2) 14_554 . . . ?
Ca2 V2 O8 Ca4 147.2(2) 14_554 . . . ?
Ca2 V3 O9 Ca1 176.98(4) 5 . . 6 ?
Ca2 V3 O9 Ca1 -63.02(4) 5 . . 5 ?
Ca2 V3 O9 Ca1 56.98(4) 5 . . . ?
Ca2 V3 O9 Ca1 56.98(4) 6 . . 5 ?
Ca2 V3 O9 Ca1 176.98(4) 6 . . . ?
Ca2 V3 O9 Ca1 -63.02(4) 6 . . 6 ?
Ca2 V3 O10 Ca1 -65.77(11) 6 . . 5 ?
Ca2 V3 O10 Ca1 93.6(4) 5 . . 5 ?
Ca2 V3 O10 Ca2 -159.4(4) 6 . . 5 ?
Ca2 V3 O10 Ca3 10.0(6) 6 . . 10_554 ?
Ca2 V3 O10 Ca3 169.4(9) 5 . . 10_554 ?
Ca2 V3 O10 Ca5 -124.1(5) 5 . . . ?
Ca2 V3 O10 Ca5 -100.6(5) 5 . . 6 ?
Ca2 V3 O10 Ca5 100.0(3) 6 . . 6 ?
Ca2 V3 O10 Ca5 76.5(3) 6 . . . ?
Ca3 V2 O5 Ca1 -64.0(3) 5_665 . . 5_665 ?
Ca3 V2 O5 Ca1 -175.86(8) 5_665 . . 6_665 ?
Ca3 V2 O5 Ca1 81.6(2) . . . 6_665 ?
Ca3 V2 O5 Ca1 -166.59(10) . . . 5_665 ?
Ca3 V2 O5 Ca2 65.9(6) 5_665 . . 6_665 ?
Ca3 V2 O5 Ca2 -36.7(7) . . . 6_665 ?
Ca3 V2 O6 Ca1 -137.4(3) . . . 6_665 ?
Ca3 V2 O6 Ca1 178.71(13) 5_665 . . 6_665 ?
Ca3 V2 O6 Ca2 54.5(6) 5_665 . . 14_554 ?
Ca3 V2 O6 Ca2 98.4(3) . . . 14_554 ?
Ca3 V2 O6 Ca3 -43.9(4) 5_665 . . . ?
Ca3 V2 O6 Ca5 -107.2(6) 5_665 . . 16_554 ?
Ca3 V2 O6 Ca5 -63.3(6) . . . 16_554 ?
Ca3 V2 O7 Ca1 165.40(10) . . . 5_665 ?
Ca3 V2 O7 Ca1 107.3(3) 5_665 . . 5_665 ?
Ca3 V2 O7 Ca2 -29.5(13) . . . 16_654 ?
Ca3 V2 O7 Ca2 -87.6(10) 5_665 . . 16_654 ?
Ca3 V2 O7 Ca3 58.1(4) . . . 5_665 ?
Ca3 V2 O8 Ca3 -144.6(3) . . . 5_665 ?
Ca3 V2 O8 Ca3 144.6(3) 5_665 . . . ?
Ca3 V2 O8 Ca4 -108.3(3) 5_665 . . . ?
Ca3 V2 O8 Ca4 107.1(3) . . . . ?
Ca4 V1 O1 Ca1 -111.8(3) . . . . ?
Ca4 V1 O1 Ca3 27.7(6) . . . . ?
Ca4 V1 O1 Ca5 141.0(6) . . . 16_554 ?
Ca4 V1 O1 Ca5 168.3(5) . . . 14_554 ?
Ca4 V1 O1 Ca5A 158.4(16) . . . 14_554 ?
Ca4 V1 O2 Ca1 -58.1(6) . . . 6_665 ?
Ca4 V1 O2 Ca2 33.7(2) . . . 6_665 ?
Ca4 V1 O2 Ca3 111.1(5) . . . 8_554 ?
Ca4 V1 O2 Ca5 -111.6(3) . . . 16_554 ?
Ca4 V1 O2 Ca5A -128(3) . . . 14_554 ?
Ca4 V1 O3 Ca1 86.85(17) . . . . ?
Ca4 V1 O3 Ca2 -20.4(2) . . . 5 ?
Ca4 V1 O3 Ca3 -155.5(3) . . . 9_454 ?
Ca4 V1 O4 Ca2 105.8(5) . . . 5 ?
Ca4 V1 O4 Ca2 -124.6(7) . . . 6_665 ?
Ca4 V2 O5 Ca1 129.12(19) . . . 6_665 ?
Ca4 V2 O5 Ca1 -119.0(2) . . . 5_665 ?
Ca4 V2 O5 Ca2 10.9(6) . . . 6_665 ?
Ca4 V2 O6 Ca1 -102.2(2) . . . 6_665 ?
Ca4 V2 O6 Ca2 133.6(3) . . . 14_554 ?
Ca4 V2 O6 Ca3 35.2(2) . . . . ?
Ca4 V2 O6 Ca5 -28.1(6) . . . 16_554 ?
Ca4 V2 O7 Ca1 84.5(3) . . . 5_665 ?
Ca4 V2 O7 Ca2 -110.4(10) . . . 16_654 ?
Ca4 V2 O7 Ca3 -22.8(3) . . . 5_665 ?
Ca4 V2 O8 Ca3 -107.1(3) . . . . ?
Ca4 V2 O8 Ca3 108.3(3) . . . 5_665 ?
Ca5 V1 O1 Ca1 79.9(6) 14_554 . . . ?
Ca5 V1 O1 Ca1 107.2(7) 16_554 . . . ?
Ca5 V1 O1 Ca3 -113.3(9) 16_554 . . . ?
Ca5 V1 O1 Ca3 -140.6(9) 14_554 . . . ?
Ca5 V1 O1 Ca5 -27.3(7) 14_554 . . 16_554 ?
Ca5 V1 O1 Ca5 27.3(7) 16_554 . . 14_554 ?
Ca5 V1 O2 Ca1 66.8(5) 14_554 . . 6_665 ?
Ca5 V1 O2 Ca1 53.5(5) 16_554 . . 6_665 ?
Ca5 V1 O2 Ca2 145.2(3) 16_554 . . 6_665 ?
Ca5 V1 O2 Ca2 158.6(2) 14_554 . . 6_665 ?
Ca5 V1 O2 Ca3 -137.3(7) 16_554 . . 8_554 ?
Ca5 V1 O2 Ca3 -124.0(6) 14_554 . . 8_554 ?
Ca5 V1 O2 Ca5 13.3(3) 14_554 . . 16_554 ?
Ca5 V1 O3 Ca1 -40.7(3) 14_554 . . . ?
Ca5 V1 O3 Ca1 -47.8(3) 16_554 . . . ?
Ca5 V1 O3 Ca2 -147.9(3) 14_554 . . 5 ?
Ca5 V1 O3 Ca2 -155.0(2) 16_554 . . 5 ?
Ca5 V1 O3 Ca3 69.9(5) 16_554 . . 9_454 ?
Ca5 V1 O3 Ca3 77.0(4) 14_554 . . 9_454 ?
Ca5 V1 O4 Ca2 146.8(4) 16_554 . . 5 ?
Ca5 V1 O4 Ca2 114.1(8) 14_554 . . 5 ?
Ca5 V1 O4 Ca2 -116.3(7) 14_554 . . 6_665 ?
Ca5 V1 O4 Ca2 -83.6(7) 16_554 . . 6_665 ?
Ca5 V1 O4 Ca4 8.4(11) 14_554 . . . ?
Ca5 V1 O4 Ca4 41.0(8) 16_554 . . . ?
Ca5 V3 O9 Ca1 -80.4(9) 5 . . . ?
Ca5 V3 O9 Ca1 39.6(9) 5 . . 6 ?
Ca5 V3 O9 Ca1 -80.4(9) 6 . . 5 ?
Ca5 V3 O9 Ca1 159.6(9) . . . . ?
Ca5 V3 O9 Ca1 39.6(9) . . . 5 ?
Ca5 V3 O9 Ca1 159.6(9) 6 . . 6 ?
Ca5 V3 O9 Ca1 159.6(9) 5 . . 5 ?
Ca5 V3 O9 Ca1 -80.4(9) . . . 6 ?
Ca5 V3 O9 Ca1 39.6(9) 6 . . . ?
Ca5 V3 O10 Ca1 -142.3(4) . . . 5 ?
Ca5 V3 O10 Ca1 -157.1(2) 5 . . 5 ?
Ca5 V3 O10 Ca1 -165.8(3) 6 . . 5 ?
Ca5 V3 O10 Ca2 124.1(5) . . . 5 ?
Ca5 V3 O10 Ca2 100.6(5) 6 . . 5 ?
Ca5 V3 O10 Ca2 109.3(4) 5 . . 5 ?
Ca5 V3 O10 Ca3 -66.5(6) . . . 10_554 ?
Ca5 V3 O10 Ca3 -81.4(6) 5 . . 10_554 ?
Ca5 V3 O10 Ca3 -90.0(7) 6 . . 10_554 ?
Ca5 V3 O10 Ca5 8.7(4) 5 . . 6 ?
Ca5 V3 O10 Ca5 -23.5(6) 6 . . . ?
Ca5 V3 O10 Ca5 -14.8(5) 5 . . . ?
Ca5 V3 O10 Ca5 23.5(6) . . . 6 ?
O1 V1 O2 Ca1 35.8(7) . . . 6_665 ?
O1 V1 O2 Ca2 127.6(5) . . . 6_665 ?
O1 V1 O2 Ca3 -155.0(6) . . . 8_554 ?
O1 V1 O2 Ca5 -17.7(6) . . . 16_554 ?
O1 V1 O2 Ca5A -34(3) . . . 14_554 ?
O1 V1 O3 Ca1 0.1(4) . . . . ?
O1 V1 O3 Ca2 -107.1(4) . . . 5 ?
O1 V1 O3 Ca3 117.7(5) . . . 9_454 ?
O1 V1 O4 Ca2 -129.7(5) . . . 6_665 ?
O1 V1 O4 Ca2 100.7(4) . . . 5 ?
O1 V1 O4 Ca4 -5.1(6) . . . . ?
O2 V1 O1 Ca1 130.8(3) . . . . ?
O2 V1 O1 Ca3 -89.7(7) . . . . ?
O2 V1 O1 Ca5 50.9(7) . . . 14_554 ?
O2 V1 O1 Ca5 23.6(7) . . . 16_554 ?
O2 V1 O1 Ca5A 41.0(17) . . . 14_554 ?
O2 V1 O3 Ca1 -128.6(4) . . . . ?
O2 V1 O3 Ca2 124.2(3) . . . 5 ?
O2 V1 O3 Ca3 -10.9(6) . . . 9_454 ?
O2 V1 O4 Ca2 -133.7(3) . . . 5 ?
O2 V1 O4 Ca2 -4.1(5) . . . 6_665 ?
O2 V1 O4 Ca4 120.6(4) . . . . ?
O3 V1 O1 Ca1 -0.1(4) . . . . ?
O3 V1 O1 Ca3 139.4(6) . . . . ?
O3 V1 O1 Ca5 -107.3(5) . . . 16_554 ?
O3 V1 O1 Ca5 -80.0(5) . . . 14_554 ?
O3 V1 O1 Ca5A -89.9(16) . . . 14_554 ?
O3 V1 O2 Ca1 159.2(4) . . . 6_665 ?
O3 V1 O2 Ca2 -109.0(2) . . . 6_665 ?
O3 V1 O2 Ca3 -31.6(7) . . . 8_554 ?
O3 V1 O2 Ca5 105.7(4) . . . 16_554 ?
O3 V1 O2 Ca5A 89(3) . . . 14_554 ?
O3 V1 O4 Ca2 119.7(4) . . . 6_665 ?
O3 V1 O4 Ca2 -9.8(3) . . . 5 ?
O3 V1 O4 Ca4 -115.6(4) . . . . ?
O4 V1 O1 Ca1 -109.1(4) . . . . ?
O4 V1 O1 Ca3 30.3(8) . . . . ?
O4 V1 O1 Ca5 143.7(6) . . . 16_554 ?
O4 V1 O1 Ca5 171.0(5) . . . 14_554 ?
O4 V1 O1 Ca5A 161.1(16) . . . 14_554 ?
O4 V1 O2 Ca1 -88.7(5) . . . 6_665 ?
O4 V1 O2 Ca2 3.0(4) . . . 6_665 ?
O4 V1 O2 Ca3 80.5(7) . . . 8_554 ?
O4 V1 O2 Ca5 -142.2(4) . . . 16_554 ?
O4 V1 O2 Ca5A -159(3) . . . 14_554 ?
O4 V1 O3 Ca1 117.5(3) . . . . ?
O4 V1 O3 Ca2 10.3(3) . . . 5 ?
O4 V1 O3 Ca3 -124.8(4) . . . 9_454 ?
O5 V2 O6 Ca1 -17.9(4) . . . 6_665 ?
O5 V2 O6 Ca2 -142.1(4) . . . 14_554 ?
O5 V2 O6 Ca3 119.5(3) . . . . ?
O5 V2 O6 Ca5 56.2(7) . . . 16_554 ?
O5 V2 O7 Ca1 0.3(4) . . . 5_665 ?
O5 V2 O7 Ca2 165.3(10) . . . 16_654 ?
O5 V2 O7 Ca3 -107.1(3) . . . 5_665 ?
O5 V2 O8 Ca3 99.4(3) . . . 5_665 ?
O5 V2 O8 Ca3 -116.0(3) . . . . ?
O5 V2 O8 Ca4 -8.9(4) . . . . ?
O6 V2 O5 Ca1 127.5(3) . . . 5_665 ?
O6 V2 O5 Ca1 15.7(4) . . . 6_665 ?
O6 V2 O5 Ca2 -102.6(6) . . . 6_665 ?
O6 V2 O7 Ca1 -119.6(3) . . . 5_665 ?
O6 V2 O7 Ca2 45.5(12) . . . 16_654 ?
O6 V2 O7 Ca3 133.1(3) . . . 5_665 ?
O6 V2 O8 Ca3 -142.6(3) . . . 5_665 ?
O6 V2 O8 Ca3 2.0(3) . . . . ?
O6 V2 O8 Ca4 109.1(3) . . . . ?
O7 V2 O5 Ca1 -0.3(4) . . . 5_665 ?
O7 V2 O5 Ca1 -112.1(3) . . . 6_665 ?
O7 V2 O5 Ca2 129.6(7) . . . 6_665 ?
O7 V2 O6 Ca1 100.7(4) . . . 6_665 ?
O7 V2 O6 Ca2 -23.5(6) . . . 14_554 ?
O7 V2 O6 Ca3 -121.9(4) . . . . ?
O7 V2 O6 Ca5 174.8(5) . . . 16_554 ?
O7 V2 O8 Ca3 130.7(4) . . . . ?
O7 V2 O8 Ca3 -13.8(4) . . . 5_665 ?
O7 V2 O8 Ca4 -122.2(4) . . . . ?
O8 V2 O5 Ca1 -113.8(3) . . . 5_665 ?
O8 V2 O5 Ca1 134.3(2) . . . 6_665 ?
O8 V2 O5 Ca2 16.0(7) . . . 6_665 ?
O8 V2 O6 Ca1 -139.1(3) . . . 6_665 ?
O8 V2 O6 Ca2 96.7(4) . . . 14_554 ?
O8 V2 O6 Ca3 -1.7(3) . . . . ?
O8 V2 O6 Ca5 -65.0(6) . . . 16_554 ?
O8 V2 O7 Ca1 118.7(3) . . . 5_665 ?
O8 V2 O7 Ca2 -76.2(11) . . . 16_654 ?
O8 V2 O7 Ca3 11.4(3) . . . 5_665 ?
O9 V3 O10 Ca1 24.97(17) . . . 5 ?
O9 V3 O10 Ca2 -68.7(4) . . . 5 ?
O9 V3 O10 Ca3 100.7(6) . . . 10_554 ?
O9 V3 O10 Ca5 -169.2(3) . . . 6 ?
O9 V3 O10 Ca5 167.2(3) . . . . ?
O10 V3 O9 Ca1 -149.9(2) 5 . . . ?
O10 V3 O9 Ca1 90.1(2) . . . . ?
O10 V3 O9 Ca1 90.1(2) 5 . . 5 ?
O10 V3 O9 Ca1 -149.9(2) . . . 6 ?
O10 V3 O9 Ca1 -149.9(2) 6 . . 5 ?
O10 V3 O9 Ca1 -29.9(2) 6 . . . ?
O10 V3 O9 Ca1 -29.9(2) . . . 5 ?
O10 V3 O9 Ca1 90.1(2) 6 . . 6 ?
O10 V3 O9 Ca1 -29.9(2) 5 . . 6 ?
O10 V3 O10 Ca1 141.6(3) 6 . . 5 ?
O10 V3 O10 Ca1 -91.6(4) 5 . . 5 ?
O10 V3 O10 Ca2 47.9(7) 6 . . 5 ?
O10 V3 O10 Ca2 174.75(18) 5 . . 5 ?
O10 V3 O10 Ca3 -142.7(3) 6 . . 10_554 ?
O10 V3 O10 Ca3 -15.9(9) 5 . . 10_554 ?
O10 V3 O10 Ca5 -52.6(5) 6 . . 6 ?
O10 V3 O10 Ca5 74.2(4) 5 . . 6 ?
O10 V3 O10 Ca5 -76.2(5) 6 . . . ?
O10 V3 O10 Ca5 50.6(5) 5 . . . ?
Ca5A V1 O1 Ca1 89.8(16) 14_554 . . . ?
Ca5A V1 O1 Ca3 -130.8(17) 14_554 . . . ?
Ca5A V1 O2 Ca1 70(3) 14_554 . . 6_665 ?
Ca5A V1 O2 Ca2 162(3) 14_554 . . 6_665 ?
Ca5A V1 O2 Ca3 -121(3) 14_554 . . 8_554 ?
Ca5A V1 O3 Ca1 -55(3) 14_554 . . . ?
Ca5A V1 O3 Ca2 -162(3) 14_554 . . 5 ?
Ca5A V1 O3 Ca3 63(3) 14_554 . . 9_454 ?
Ca5A V1 O4 Ca2 148(6) 14_554 . . 5 ?
Ca5A V1 O4 Ca2 -82(6) 14_554 . . 6_665 ?
Ca5A V1 O4 Ca4 42(6) 14_554 . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.61(6)
2 0.39(6)


